#------------------------------------------------------------------------------
#$Date: 2017-02-07 17:13:06 +0200 (Tue, 07 Feb 2017) $
#$Revision: 191892 $
#$URL: file:///home/coder/svn-repositories/cod/cif/2/10/35/2103530.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided by IUCr Journals, http://journals.iucr.org/.
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_2103530
loop_
_publ_author_name
'Pavlovska, A.'
'Werner, S.'
'Maximov, B.'
'Mill, B.'
_publ_section_title
;
 Pressure-induced phase transitions of piezoelectric single crystals
 from the langasite family: La₃Nb~0.5~Ga~5.5~O₁₄ and
 La₃Ta~0.5~Ga~5.5~O₁₄
;
_journal_issue                   6
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              939
_journal_page_last               947
_journal_paper_doi               10.1107/S0108768102010273
_journal_volume                  58
_journal_year                    2002
_chemical_formula_sum            'Ga5.54 La3 O14 Ta0.46'
_chemical_formula_weight         1110.22
_chemical_name_systematic        ?
_space_group_IT_number           150
_symmetry_space_group_name_Hall  'P 3 2"'
_symmetry_space_group_name_H-M   'P 3 2 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            1
_cell_length_a                   8.155
_cell_length_b                   8.155
_cell_length_c                   5.091
_cell_measurement_temperature    293(2)
_cell_volume                     293.2
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_pressure         3.3E+6
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.598
_diffrn_measured_fraction_theta_max 0.598
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0631
_diffrn_reflns_av_sigmaI/netI    0.0386
_diffrn_reflns_limit_h_max       10
_diffrn_reflns_limit_h_min       -10
_diffrn_reflns_limit_k_max       11
_diffrn_reflns_limit_k_min       -11
_diffrn_reflns_limit_l_max       4
_diffrn_reflns_limit_l_min       -4
_diffrn_reflns_number            1624
_diffrn_reflns_theta_full        32.00
_diffrn_reflns_theta_max         32.00
_diffrn_reflns_theta_min         2.88
_exptl_absorpt_coefficient_mu    27.532
_exptl_crystal_density_diffrn    6.287
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             488
_refine_diff_density_max         1.600
_refine_diff_density_min         -1.269
_refine_diff_density_rms         0.360
_refine_ls_abs_structure_details 'Flack H D (1983), Acta Cryst. A39, 876-881'
_refine_ls_abs_structure_Flack   -0.01(6)
_refine_ls_extinction_coef       0.142(14)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.038
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     39
_refine_ls_number_reflns         433
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.038
_refine_ls_R_factor_all          0.0376
_refine_ls_R_factor_gt           0.0373
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.1000P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1082
_refine_ls_wR_factor_ref         0.1088
_reflns_number_gt                431
_reflns_number_total             433
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            sn0021-3.3cad4.cif
_cod_data_source_block           3.3cad4
_cod_depositor_comments
;
The _diffrn_ambient_pressure was taken from the original data block
header, after comparison with the paper text and supplementary
material.

Saulius Gra\<zulis
;
_cod_database_code               2103530
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'y, x, -z'
'-y, x-y, z'
'-x+y, -x, z'
'-x, -x+y, -z'
'x-y, -y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
La La 0.42716(12) 0.0000 0.0000 0.0224(4) Uani 1 2 d S
Ga1 Ga 0.0000 0.0000 0.0000 0.0239(6) Uani 0.50 6 d SP
Ta Ta 0.0000 0.0000 0.0000 0.0239(6) Uani 0.50 6 d SP
Ga2 Ga 0.6667 0.3333 0.4680(8) 0.0243(8) Uani 1 3 d S
Ga3 Ga 0.7636(2) 0.0000 0.5000 0.0245(6) Uani 1 2 d S
O1 O 0.3333 -0.3333 0.163(5) 0.030(5) Uani 1 3 d S
O2 O 0.5468(14) -0.1479(12) -0.301(3) 0.027(3) Uani 1 1 d .
O3 O 0.7831(12) -0.1433(14) 0.240(2) 0.027(3) Uani 1 1 d .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
La La -0.2871 2.4523 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ta Ta -0.7052 6.5227 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ga Ga 0.2307 1.6083 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O3 La O3 66.7(6) 5_665 3_545
O3 La O2 140.1(4) 5_665 6
O3 La O2 108.4(4) 3_545 6
O3 La O2 108.4(4) 5_665 .
O3 La O2 140.1(4) 3_545 .
O2 La O2 99.2(6) 6 .
O3 La O1 123.7(3) 5_665 .
O3 La O1 80.3(4) 3_545 .
O2 La O1 92.3(4) 6 .
O2 La O1 70.1(5) . .
O3 La O1 80.3(4) 5_665 2_655
O3 La O1 123.7(3) 3_545 2_655
O2 La O1 70.1(5) 6 2_655
O2 La O1 92.3(4) . 2_655
O1 La O1 153.23(9) . 2_655
O3 La O2 65.6(4) 5_665 3_545
O3 La O2 78.8(4) 3_545 3_545
O2 La O2 154.28(14) 6 3_545
O2 La O2 64.6(4) . 3_545
O1 La O2 64.1(5) . 3_545
O1 La O2 127.3(5) 2_655 3_545
O3 La O2 78.8(4) 5_665 5_665
O3 La O2 65.6(4) 3_545 5_665
O2 La O2 64.6(4) 6 5_665
O2 La O2 154.28(14) . 5_665
O1 La O2 127.3(5) . 5_665
O1 La O2 64.1(5) 2_655 5_665
O2 La O2 137.3(4) 3_545 5_665
O3 La Ga2 110.6(3) 5_665 .
O3 La Ga2 86.6(3) 3_545 .
O2 La Ga2 31.7(2) 6 .
O2 La Ga2 128.6(3) . .
O1 La Ga2 111.6(5) . .
O1 La Ga2 63.4(5) 2_655 .
O2 La Ga2 165.2(2) 3_545 .
O2 La Ga2 32.9(2) 5_665 .
O3 La Ga2 86.6(3) 5_665 2_545
O3 La Ga2 110.6(3) 3_545 2_545
O2 La Ga2 128.6(3) 6 2_545
O2 La Ga2 31.7(2) . 2_545
O1 La Ga2 63.4(5) . 2_545
O1 La Ga2 111.6(5) 2_655 2_545
O2 La Ga2 32.9(2) 3_545 2_545
O2 La Ga2 165.2(2) 5_665 2_545
Ga2 La Ga2 159.89(4) . 2_545
O3 La Ga1 33.4(3) 5_665 .
O3 La Ga1 33.4(3) 3_545 .
O2 La Ga1 130.4(3) 6 .
O2 La Ga1 130.4(3) . .
O1 La Ga1 103.38(5) . .
O1 La Ga1 103.38(5) 2_655 .
O2 La Ga1 68.7(2) 3_545 .
O2 La Ga1 68.7(2) 5_665 .
Ga2 La Ga1 100.057(18) . .
Ga2 La Ga1 100.058(18) 2_545 .
O3 La Ta 33.4(3) 5_665 .
O3 La Ta 33.4(3) 3_545 .
O2 La Ta 130.4(3) 6 .
O2 La Ta 130.4(3) . .
O1 La Ta 103.38(5) . .
O1 La Ta 103.38(5) 2_655 .
O2 La Ta 68.7(2) 3_545 .
O2 La Ta 68.7(2) 5_665 .
Ga2 La Ta 100.057(18) . .
Ga2 La Ta 100.058(18) 2_545 .
Ga1 La Ta 0.0 . .
O3 Ga1 O3 86.0(4) 2_545 5_665
O3 Ga1 O3 106.5(6) 2_545 3_545
O3 Ga1 O3 84.1(5) 5_665 3_545
O3 Ga1 O3 86.0(4) 2_545 6_455
O3 Ga1 O3 86.0(4) 5_665 6_455
O3 Ga1 O3 163.5(6) 3_545 6_455
O3 Ga1 O3 84.1(5) 2_545 1_455
O3 Ga1 O3 163.5(6) 5_665 1_455
O3 Ga1 O3 86.0(4) 3_545 1_455
O3 Ga1 O3 106.5(6) 6_455 1_455
O3 Ga1 O3 163.5(6) 2_545 4_665
O3 Ga1 O3 106.5(6) 5_665 4_665
O3 Ga1 O3 86.0(4) 3_545 4_665
O3 Ga1 O3 84.1(5) 6_455 4_665
O3 Ga1 O3 86.0(4) 1_455 4_665
O3 Ga1 La 42.1(3) 2_545 4
O3 Ga1 La 126.8(3) 5_665 4
O3 Ga1 La 98.3(3) 3_545 4
O3 Ga1 La 98.3(3) 6_455 4
O3 Ga1 La 42.1(3) 1_455 4
O3 Ga1 La 126.8(3) 4_665 4
O3 Ga1 La 98.3(3) 2_545 .
O3 Ga1 La 42.1(3) 5_665 .
O3 Ga1 La 42.1(3) 3_545 .
O3 Ga1 La 126.8(3) 6_455 .
O3 Ga1 La 126.8(3) 1_455 .
O3 Ga1 La 98.3(3) 4_665 .
La Ga1 La 120.0 4 .
O3 Ga1 La 126.8(3) 2_545 2
O3 Ga1 La 98.3(3) 5_665 2
O3 Ga1 La 126.8(3) 3_545 2
O3 Ga1 La 42.1(3) 6_455 2
O3 Ga1 La 98.3(3) 1_455 2
O3 Ga1 La 42.1(3) 4_665 2
La Ga1 La 120.0 4 2
La Ga1 La 120.0 . 2
O3 Ta O3 86.0(4) 2_545 5_665
O3 Ta O3 106.5(6) 2_545 3_545
O3 Ta O3 84.1(5) 5_665 3_545
O3 Ta O3 86.0(4) 2_545 6_455
O3 Ta O3 86.0(4) 5_665 6_455
O3 Ta O3 163.5(6) 3_545 6_455
O3 Ta O3 84.1(5) 2_545 1_455
O3 Ta O3 163.5(6) 5_665 1_455
O3 Ta O3 86.0(4) 3_545 1_455
O3 Ta O3 106.5(6) 6_455 1_455
O3 Ta O3 163.5(6) 2_545 4_665
O3 Ta O3 106.5(6) 5_665 4_665
O3 Ta O3 86.0(4) 3_545 4_665
O3 Ta O3 84.1(5) 6_455 4_665
O3 Ta O3 86.0(4) 1_455 4_665
O3 Ta La 42.1(3) 2_545 4
O3 Ta La 126.8(3) 5_665 4
O3 Ta La 98.3(3) 3_545 4
O3 Ta La 98.3(3) 6_455 4
O3 Ta La 42.1(3) 1_455 4
O3 Ta La 126.8(3) 4_665 4
O3 Ta La 98.3(3) 2_545 .
O3 Ta La 42.1(3) 5_665 .
O3 Ta La 42.1(3) 3_545 .
O3 Ta La 126.8(3) 6_455 .
O3 Ta La 126.8(3) 1_455 .
O3 Ta La 98.3(3) 4_665 .
La Ta La 120.0 4 .
O3 Ta La 126.8(3) 2_545 2
O3 Ta La 98.3(3) 5_665 2
O3 Ta La 126.8(3) 3_545 2
O3 Ta La 42.1(3) 6_455 2
O3 Ta La 98.3(3) 1_455 2
O3 Ta La 42.1(3) 4_665 2
La Ta La 120.0 4 2
La Ta La 120.0 . 2
O2 Ga2 O2 100.5(5) 6 2_655
O2 Ga2 O2 100.5(5) 6 5_665
O2 Ga2 O2 100.5(5) 2_655 5_665
O2 Ga2 O1 117.4(4) 6 2_656
O2 Ga2 O1 117.4(4) 2_655 2_656
O2 Ga2 O1 117.4(4) 5_665 2_656
O2 Ga2 La 43.9(3) 6 .
O2 Ga2 La 107.7(4) 2_655 .
O2 Ga2 La 56.6(4) 5_665 .
O1 Ga2 La 134.46(5) 2_656 .
O2 Ga2 La 56.6(4) 6 2_655
O2 Ga2 La 43.9(3) 2_655 2_655
O2 Ga2 La 107.7(5) 5_665 2_655
O1 Ga2 La 134.46(5) 2_656 2_655
La Ga2 La 76.36(7) . 2_655
O2 Ga2 La 107.7(4) 6 4_665
O2 Ga2 La 56.6(4) 2_655 4_665
O2 Ga2 La 43.9(3) 5_665 4_665
O1 Ga2 La 134.46(5) 2_656 4_665
La Ga2 La 76.36(7) . 4_665
La Ga2 La 76.36(7) 2_655 4_665
O3 Ga3 O3 132.0(5) . 6_556
O3 Ga3 O2 109.8(5) . 1_556
O3 Ga3 O2 99.8(5) 6_556 1_556
O3 Ga3 O2 99.8(5) . 6
O3 Ga3 O2 109.8(5) 6_556 6
O2 Ga3 O2 102.7(7) 1_556 6
Ga2 O1 La 108.9(5) 2_546 .
Ga2 O1 La 108.9(5) 2_546 4_655
La O1 La 110.0(5) . 4_655
Ga2 O1 La 108.9(5) 2_546 2_545
La O1 La 110.0(5) . 2_545
La O1 La 110.0(5) 4_655 2_545
Ga2 O2 Ga3 118.7(7) 2_545 1_554
Ga2 O2 La 104.4(4) 2_545 .
Ga3 O2 La 120.4(4) 1_554 .
Ga2 O2 La 90.6(4) 2_545 4_655
Ga3 O2 La 112.7(4) 1_554 4_655
La O2 La 105.5(5) . 4_655
Ga3 O3 Ta 114.0(5) . 1_655
Ga3 O3 Ga1 114.0(5) . 1_655
Ta O3 Ga1 0.0 1_655 1_655
Ga3 O3 La 137.2(5) . 4_655
Ta O3 La 104.6(5) 1_655 4_655
Ga1 O3 La 104.6(5) 1_655 4_655
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
La O3 2.412(8) 5_665
La O3 2.412(8) 3_545
La O2 2.436(10) 6
La O2 2.436(10) .
La O1 2.567(8) .
La O1 2.567(8) 2_655
La O2 2.839(12) 3_545
La O2 2.839(12) 5_665
La Ga2 3.402(3) .
La Ga2 3.402(3) 2_545
La Ga1 3.4835(10) .
La Ta 3.4835(10) .
Ga1 O3 1.979(11) 2_545
Ga1 O3 1.979(11) 5_665
Ga1 O3 1.979(11) 3_545
Ga1 O3 1.979(11) 6_455
Ga1 O3 1.979(11) 1_455
Ga1 O3 1.979(11) 4_665
Ga1 La 3.4835(10) 4
Ga1 La 3.4836(10) 2
Ta O3 1.979(11) 2_545
Ta O3 1.979(11) 5_665
Ta O3 1.979(11) 3_545
Ta O3 1.979(11) 6_455
Ta O3 1.979(11) 1_455
Ta O3 1.979(11) 4_665
Ta La 3.4835(10) 4
Ta La 3.4836(10) 2
Ga2 O2 1.846(11) 6
Ga2 O2 1.846(11) 2_655
Ga2 O2 1.846(11) 5_665
Ga2 O1 1.88(2) 2_656
Ga2 La 3.402(3) 2_655
Ga2 La 3.402(3) 4_665
Ga3 O3 1.826(11) .
Ga3 O3 1.826(11) 6_556
Ga3 O2 1.864(11) 1_556
Ga3 O2 1.864(11) 6
O1 Ga2 1.88(2) 2_546
O1 La 2.567(8) 4_655
O1 La 2.567(8) 2_545
O2 Ga2 1.846(11) 2_545
O2 Ga3 1.864(11) 1_554
O2 La 2.839(12) 4_655
O3 Ta 1.979(11) 1_655
O3 Ga1 1.979(11) 1_655
O3 La 2.412(8) 4_655
